**QUANTIFICATION OF PERFORATION RESISTANCE OF **

**PRE-STRESSED WALLS WITH TRANSVERSE REINFORCEMENT AND **

**LINER UNDER HARD MISSILE IMPACT BASED ON TEST RESULTS **

**Mathieu Galan1, Nebojsa Orbovic2 **

1 _{Structural Engineer, EDF (Nuclear Basic Design Department), France }
2

Technical Specialist, Canadian Nuclear Safety Commission (CNSC-CCSN), Canada

**ABSTRACT **

Based on impact of hard missiles on concrete targets test results, the increase of perforation resistance of various slabs configurations, in comparison with reinforced concrete walls is assessed. Five impact tests on reinforced concrete slabs with bending reinforcement only are used as a “baseline” result of perforation capacity of reinforced concrete slabs. The paper shows that experimental scattering is not significant for the 5 considered impact tests on reinforced concrete slabs with a variation of +/- 5 % around the calculated “experimental just-perforation velocity” mean value. A step-by-step demonstration is then proposed in order to gradually assess the increase of resistance due to each experimental parameter (transverse reinforcement, prestressing, and combination of transverse reinforcement, prestressing and liner). Perforation capacity of the reinforced concrete slab is not increased due to the presence of transverse reinforcement. This observation is due to the much localized hard impact scenario, implying a particular rupture mode of the slab for which the role of transverse reinforcement is not significant. An increase of perforation capacity can be identified in this paper, due to a 10 MPa prestressing of the slab (+10 % to + 15%) and due to the combination of a 10 MPa prestressing in the concrete, the presence of transverse reinforcement and liner (+20 % to + 25 %). This paper completes the observations made in Orbovic et al. (2009), (2011), (2013) and (2015).

**INTRODUCTION **

The hard impact tests presented in this paper were carried out at VTT test facility in Espoo, Finland. The present analysis is a continuation of the work performed in previous SMIRT papers, providing detailed insight in the phenomena related to hard impact on civil structures and their consequences. In this paper, additional results and analyses are presented.

Based on impact of hard missiles on concrete targets test results, the purpose of this paper is to quantify the increase of perforation resistance of pre-stressed walls with transverse reinforcement and liner, in comparison with reinforced concrete walls. Five impact tests on reinforced concrete slabs with bending reinforcement only (A21, A12 and the three punching tests performed during 2010 OECD_IRIS campaign P1, P2 and P3) are used as a “baseline” result of perforation capacity of reinforced concrete slabs. A21 is not described in detail because it is already presented in Orbovic et al. (2015). A step-by-step demonstration is proposed in order to gradually assess the increase of resistance due to each experimental parameter. For this purpose, the following impact tests, having the same set-up and design of the slabs, are also exploited:

- specimen P6 for which transverse reinforcement (T-headed bars) is added; - specimen C2 for which a 10 MPa pre-stressing (ungrouted tendons) is added;

- specimen CTL3 for which a combination of a 10 MPa pre-stressing (ungrouted tendons), transverse reinforcement (T-headed bars) and liner are added.

In all these impact tests, perforation of the slab was achieved, that is to say that the missile passes through the slab with a residual velocity superior to 0. This choice will allow:

- calculating an “experimental just-perforation velocity” based on the measured impact and residual velocities;

**TEST SPECIMENS **

The specimens which are analyzed in this paper have the following common characteristics:

- the projectile is hard cylindrical missile, constituted of a full of concrete 12.5 mm thick steel pipe, welded to a 50 mm thick steel dome (see Figure 1). This projectile has a constant 0.168 m diameter. Its mass is 47.5 kg;

- 2.1m*2.1m square reinforced concrete walls having a 0.25m thickness are used. The slabs are 2-ways simply supported, the supporting span being around 2.0 m in each direction (see Figure 2); - Bending reinforcement layers whose characteristics are Φ10mm@90mm each way each face (i.e.

8.7 cm²/ml ew/ef leading to a 0.35 % reinforcement ratio ew/ef) are put in place (see Figure 2). The yield strength of steel is 500 MPa.

Figure 1. Hard missile used in the tests

### Figure 2.

Baseline reinforced concrete specimen and reinforcement detailsThe slabs described in Figure 2 correspond to the ones of “baseline” specimen A21, A12, OECD IRIS P1, P2 and P3) with bending reinforcement only.

Three other specimens are analyzed. In specimens where transverse reinforcement is introduced (P6 and CTL3), one T-headed bar is placed at each intersection of longitudinal reinforcement (see Figure 3). The corresponding yield strength is 500 MPa.

In specimens where a 10 MPa pre-stressing in both directions is introduced (C2, CTL3), dywidag bars are put in PVC sleeves in order to avoid bond between the concrete and the pre-stressing bars (see Figure 3). The ultimate stress of the bars is fpu = 1030 MPa. The bars are anchored with external anchors.

The concrete compressive strength of specimens, casted at different times from different batches can vary
(see **Table 1**).

Figure 3. Description of pre-stressing rebars used in tests C2 and CTL3 and transverse reinforcement used in tests P6 and CTL3

Figure 4. Description of the liner used in test CTL3

A synthesis table of the analyzed impact tests is given below:

Table 1 : description of the impact tests

**Test n° ** **Transverse **
**reinforcement **

**10 MPa Prestressing **

**in the concrete ** **Liner **

**Concrete **
**compression **

**strength on **
**cylinder fck [MPa] **

**Impact **
**velocity Vo **

**[m/s] **

**A12 **

Bending reinforcement only

50.3 110,2

**A21 ** 55.3 120,2

**IRIS P1 ** 60,5 135,9

**IRIS P2 ** 58,3 134,9

**IRIS P3 ** 60,5 136,5

**P6 **

T-headed bars Φ10mm@90mm

= 96.9 cm²/m²

No No 49.7 123,4

**C2 ** No

10 dywidag bars Φ26.5mm@180mm =

31.8 cm²/ml ED (non grouted tendons)

No 54,2 141,6

**CTL3 **

T-headed bars Φ12mm@90mm

= 140 cm²/m²

Same as C2 1.5 mm

**TEST RESULTS **

Each specimen is perforated after the impact. The residual velocity of the missile after perforation is
given in **Table 3**. A maximum of 2 horizontal and 2 vertical rebars (at front and rear faces of the slabs)
were broken. In tests with pre-stressing, 1 or 2 dywidag bars are broken. The parameter playing a major
role on the size of the scabbed area is transverse reinforcement ratio, as already mentioned in Orbovic et
al. (2009). The scabbing area is approximately equal to 1 m² without T-headed bars and to 0.2 to 0.4 m²
with T-headed bars.

An important point to have in mind is that in the tests chosen in this paper, the energy dissipated by
deformation of the missile was not significant (see **Table 2**). These tests can be considered as “hard
impact tests”. As a consequence, the damage of concrete slabs can be compared from one test to another,
and the influence of each parameter of the slab can be assessed.

Table 2 : Slabs and missiles after impact

**Test **

**n° ** **Front and rear faces of the slab after impact ** **Missile after impact **

**A12 **

**IRIS **
**P2 **

**P6 **

**C2 **

**CTL3 **

(*) *photos describing damage of A21 specimen are given in Orbovic et al. (2015)*

Numerical values describing main test results are given in **Table 3**:

Table 3 : Notable results of the considered impact tests

**Test n° ** **Residual velocity after **
**peforation VR [m/s] **

**Scabbing area **
**Sc [m²] **

**Broken rebars in H **
**and V directions **

**Mass of ejected **
**concrete Mc [kg] **

**A12 ** 20,8 0.972 Front: 2H 1V

Back : 1V

**A21 ** 33,4 1.028 Front: 2H 2V

Back : 1V

**IRIS P1 ** 33,8 1.055 Front: 2H 2V

Back : 1H 1V 30 – 60 kg

**IRIS P2 ** 45,8 1.0043 Front: 2H 2V

Back : 1H 2V 116 kg

**IRIS P3 ** 35,8 1.123 Front: 2H 2V

Back : 2H 1V 121 kg

**P6 ** 5,0 0.337 Front: 2H 2V

Back : 2H 2V

**C2 ** 39,0 0.999

Front: 2H 2V Back : 1H 1V Dywidag : 1H

**CTL3 ** 17,5 0.205

**PERFORATION CAPACITY OF SPECIMENS **

The energy balance of hard impact can be written as follows:

E0 = Ejp + Em + ER

Where:

- E0 = 0.5*M*V0² kinetic energy of the missile (with M and V0 respectively the mass and impact

velocity of the missile);

- Ejp = 0.5*M*Vjp² the energy necessary to just-perforate the wall with Vjp the just-perforation

velocity of the structure;

- Em the energy dissipated by deformation of the projectile. For hard missile impact, we consider

that Em ~ 0;

- ER = 0.5*(M+Mc)*VR2 residual kinetic energy of the secondary projectile (including a concrete

cone whose mass is equal to Mc) with VR its residual velocity.

Figure 5. Definition of masses and velocities in the perforation process

Ejected concrete mass Mc is supposed to be a punching cone forming an angle with the middle

plane of the slab. Its characteristic radius are R (radius of the impacting projectile) and R2=R+h*cotan(α).

The ejected mass is calculated by:

With c = 2500 kg/m3 concrete density and h the slab thickness.

Angle θ is calculated by Kar formula, as described in NEI 07-13 (2011):

Figure 6. Definition of the punching cone angle

The numerical value of angle θ for all the considered impact tests is approximately equal to 40 degrees, using Kar formula. In some of the presented impact tests (in particular the ones with transverse reinforcement), the rupture mode of the slab is not clearly a punching cone with such an angle. In these cases, the rupture mode is close to a cylinder with a slight increase of the angle at the location of rear bending reinforcement (see Figure 7), with an angle of θ close to 0° (additional analysis on this topic is given in Orbovic et al. (2013)).

Figure 7. Horizontal cross sections of slabs P6 with transverse reinforcement (on the left) and IRIS P2 without transverse reinforcement (on the right)

A sensitivity analysis is carried out on this parameter because it influences the calculation of the ejected concrete plug mass. The ejected mass Mc is 75.6 kg for θ ~ 40° and 13.9 kg for θ = 0°.

In this paper, an “experimental just-perforation velocity VJP” is estimated for a given slab configuration,

knowing the measured residual velocity of the missile after perforation VR, as:

The calculation is performed in the table below for θ = 40° and θ = 0°:

Table 4 : Calculation of "experimental just-perforation velocity" Vjp

** ** **Test data ** **Calculation for θ = 40° Calculation for θ = 0° **

**Test n° ** Impact velocity
**Vo [m/s]**

Residual velocity after perforation

**VR [m/s]**

"Experimental just-perforation velocity" **Vjp [m/s]**

**A12 ** 110,2 20,8 105,0 107,6

**A21 ** 120,2 33,4 107,5 114,0

**IRIS P1 ** 135,9 33,8 124,5 130,4

**IRIS P2 ** 134,9 45,8 113,0 124,4

**IRIS P3 ** 136,5 35,8 123,7 130,3

**P6 ** 110,7 5,0 110,4 110,6

**C2 ** 141,6 39,0 126,9 134,5

**CTL3 ** 148,8 17,5 146,1 147,5

The “experimental VJP” values given in **Table 4** cannot directly be compared between each test because

the corresponding slabs do not necessarily have the same concrete compression strength (see **Table 1**).
As a consequence, the “experimental VJP” values given in **Table 4** have to be corrected by a coefficient
taking into account this difference in the concrete compression strengths between each test.

Based on the CEA-EDF formula given in ETC-C (2012), it can be seen that the just-perforation velocity VJP is proportional to the square root of concrete compression strength:

The “experimental VJP” values given in **Table 4** are consequently corrected by the following

coefficient

. Here, we take = 50.3 MPa.

In **Table 5**, the “corrected experimental just-perforation velocities” VJP* are calculated by:

** **

The corrected VJP* values can now be compared for each test because they correspond to the same

concrete compression strength = 50.3 MPa.

Increase of perforation capacity for each slab configuration, in comparison with perforation capacity of reinforced concrete with bending reinforcement only, is then calculated by:

_{ }
_{ }

with _{ } _{ } _{ } _{ } _{ } _{ } .

The various coefficients are calculated in the following **Table 5**:

Table 5 : Corrected "experimental just-perforation velocity" Vjp*; increase of perforation capacity μi

Test data Calculation for θ = 40° Calculation for θ = 0°

Test n° fck [MPa] [m/s] **Ratio ** ** [-] ** [m/s] **Ratio ** ** [-] **

Baseline tests with reinforced concrete only **“RC”**

A12 50,3 105,0 0,97 107,6 0,94

A21 53,4 104,3 0,96 110,7 0,97

IRIS P1 60,5 113,6 1,05 118,9 1,04

IRIS P2 58,3 104,9 0,97 115,6 1,01

IRIS P3 60,5 112,8 1,04 118,8 1,04

Effect of transverse shear reinforcement **“RCT”**

P6 49,7 111,1

**1,03 **

111,2 **0,97 **

Effect of prestressing **“PC”**

C2 54,2 122,3

**1,13 **

129,5 **1,13 **

Effect of prestressing combined with transverse reinforcement and liner **“PCTL”**

CTL3 58,7 135,3

**1,25 **

136,5 **1,19 **

In **Table 5**, we can note that:

- Experimental scattering is not significant for the 5 considered impact tests on reinforced concrete
slabs with a variation of +/- 5 % of the mean value _{ }

. This observation shows the good

control of the performed impact tests and the high level of confidence of the corresponding results; - Perforation capacity of the reinforced concrete slab is not increased due to the presence of transverse

- A +10 % to +15% increase of perforation capacity can be identified in this paper, due to a 10 MPa prestressing of the slab;

- An increase of perforation capacity is observed, due to the combination of a 10 MPa prestressing in the concrete, the presence of transverse reinforcement and liner. This increase is estimated to be between +20 % to +25 %. This calculation allows quantifying the favourable effect of the combination of these parameters on perforation capacity against hard missile impact. It completes the qualitative observations made in Orbovic et al. (2011), on hard impact tests carried out at lower velocities (~100 m/s).

This increase of perforation capacity observed in test CTL3 could partly be explained by the triaxial confinement state of concrete, in both horizontal directions with prestressing and in the transverse direction with T-headed bars, which can significantly increase the concrete compression strength (see Figure 8). Another effect, due to the presence of dywidag bars into the slab, is discussed in Orbovic et al (2015) and Sagals et al (2015).

Figure 8. Triaxial tests on cylindrical concrete test pieces – input data from the OCDE_IRIS workshop 2012

Increase of concrete compression strength due to triaxial confinement can be calculated thanks to Eurocode 2 Part 1-1 (2005). By way of example, the lateral pressure σ2 considered in the calculation is the

10 MPa due to prestressing.

The increase of concrete strength

is then assessed to be 1.55 in test CTL3 (with fck = 58.7 MPa).

As the just-perforation velocity Vjp is proportional to the square root of concrete compression strength, the

increase of perforation capacity of the slab in a 10 MPa triaxial confinement state is estimated to be:

This value can be considered as consistent with the calculated +20 % to +25 % increase of perforation capacity, based on CTL3 test result. On this topic, additional investigations should be carried out in order to more precisely assess the effect of confinement on perforation capacity.

**CONCLUSION **

Based on impact of hard missiles on concrete targets test results, the increase of perforation resistance of various slabs configurations, in comparison with reinforced concrete walls is assessed. The paper shows that experimental scattering is not significant for the 5 considered impact tests on reinforced concrete slabs with bending reinforcement, with a variation of +/- 5 % around the calculated “experimental just-perforation velocity” mean value, giving a high level of confidence in the results. An increase of

perforation capacity is observed due to prestressing of the slab (+10 % to + 15%) and due to the combination of a prestressing in the concrete, the presence of transverse reinforcement and liner (+20 % to + 25 %). This increase could partly be explained by the favourable effect of concrete confinement in prestressed concrete slabs with transverse shear reinforcement.

**REFERENCES **

Eurocode 2 Partie 1-1 (2005). “Calcul des structures en béton – Partie 1.1 : Règles générales et règles pour les bâtiments”, EN 1992-1-1.

ETC-C (2012) “EPR Technical Code for Civil Works”, 2012 Edition.

NEI 07-13 (2011). “Methodology for Performing Aircraft Impact Assessments for New Plant Design”, revision 8P, ERIN Engineering & Research, Inc.

OECD/NEA Workshop IRIS_2010 (2012). “Improving Robustness Assessment Methodologies for Structures Impacted by Missiles (IRIS_2010)”. Final Report, OECD/NEA website, http://www.oecdnea.org.

OECD/NEA Workshop IRIS_2012 (2013). “ Improving Robustness Assessment Methodologies for Structures Impacted by Missiles. Draft Conclusions and Recommendations”, OECD/NEA website, http://www.oecd-nea.org.

Orbovic N., Galan M. and Blahoianu A. (2015). “Hard Missile Impact Tests in Order to Assess the Effect of Pres-stressing on Perforation Capacity” Paper presented at 23rd SMiRT, Manchester, UK. Orbovic N. and Blahoianu A. (2013). “Tests to determine the influence of transverse reinforcement on

perforation resistance of RC slabs under hard missile impact,” Paper presented at 22nd SMiRT, San Francisco, California, USA.

Orbovic, N. and Blahoianu, A. (2011). “Tests on concrete slabs under hard missile impact to evaluate the influence of transverse reinforcement and pre-stressing on perforation velocity”, SMiRT_21 Proceedings, New Delhi, India, SMiRT-21, November, 2011.

Orbovic, N., Elgohary, M., Lee, N.H., and Blahoianu, A. (2009). “Tests on Reinforced Concrete Slabs with Pre-stressing and with Transverse Reinforcement under Impact Loading” SMiRT_20 Proceedings, Espoo, Finland, SMiRT-20, August 2009.